#------------------------------------------------------------------------------
#$Date: 2024-07-05 20:24:42 +0300 (Fri, 05 Jul 2024) $
#$Revision: 293169 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/24/83/7248370.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7248370
loop_
_publ_author_name
'Li, Ke'
'Liu, Yufeng'
'Yang, Guoping'
'Zheng, Zhijian'
'Lin, Xiaoling'
'Zhang, Zhibin'
'Li, Shujun'
'Liu, Yunhai'
'Wei, Yongge'
_publ_section_title
;
 Highly-stable Silverton-type UIV-containing polyoxomolybdate frameworks
 for the heterogeneous catalytic synthesis of quinazolinones
;
_journal_issue                   11
_journal_name_full               'Green Chemistry'
_journal_page_first              6454
_journal_page_last               6460
_journal_paper_doi               10.1039/D4GC00877D
_journal_volume                  26
_journal_year                    2024
_chemical_formula_moiety         'Co1 Mo12 Na3.6 O51 U1, 4.5(O)'
_chemical_formula_sum            'Co H29.4 Mo12 Na3.6 O55.5 U'
_chemical_formula_weight         2448.64
_space_group_crystal_system      cubic
_space_group_IT_number           206
_space_group_name_Hall           '-I 2b 2c 3'
_space_group_name_H-M_alt        'I a -3'
_atom_sites_solution_primary     dual
_audit_creation_date             2023-07-20
_audit_creation_method
;
Olex2 1.5
(compiled 2023.02.24 svn.rf166f9f3 for OlexSys, GUI svn.r6725)
;
_audit_update_record
;
2023-07-20 deposited with the CCDC.	2024-04-02 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   25.9609(3)
_cell_length_b                   25.9609(3)
_cell_length_c                   25.9609(3)
_cell_measurement_reflns_used    9243
_cell_measurement_temperature    150
_cell_measurement_theta_max      25.011
_cell_measurement_theta_min      2.936
_cell_volume                     17496.8(4)
_computing_cell_refinement       'SAINT V8.38A (Bruker, 2018)'
_computing_data_reduction        'SAINT V8.38A (Bruker, 2018)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      150.00
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0383
_diffrn_reflns_av_unetI/netI     0.0198
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            25767
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.011
_diffrn_reflns_theta_max         25.011
_diffrn_reflns_theta_min         1.921
_diffrn_source_current           1.4
_diffrn_source_power             0.07
_diffrn_source_voltage           50.0
_exptl_absorpt_coefficient_mu    7.549
_exptl_absorpt_correction_T_max  0.7452
_exptl_absorpt_correction_T_min  0.6796
_exptl_absorpt_correction_type   none
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1037 before and 0.0540 after correction.
The Ratio of minimum to maximum transmission is 0.9120.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            'clear dark brown'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    brown
_exptl_crystal_density_diffrn    3.718
_exptl_crystal_description       block
_exptl_crystal_F_000             18176
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.099
_refine_diff_density_min         -0.722
_refine_diff_density_rms         0.134
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.131
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     247
_refine_ls_number_reflns         2589
_refine_ls_number_restraints     30
_refine_ls_restrained_S_all      1.129
_refine_ls_R_factor_all          0.0289
_refine_ls_R_factor_gt           0.0235
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0128P)²+294.1928P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0530
_refine_ls_wR_factor_ref         0.0549
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2303
_reflns_number_total             2589
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4gc00877d2.cif
_cod_data_source_block           Co1
_cod_depositor_comments
'Adding full bibliography for 7248368--7248371.cif.'
_cod_original_cell_volume        17496.8(6)
_cod_original_formula_sum        'Co H29.40 Mo12 Na3.60 O55.50 U'
_cod_database_code               7248370
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.583
_shelx_estimated_absorpt_t_min   0.519
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O16) \\sim Ueq, Uanis(O16A) \\sim Ueq, Uanis(O17A) \\sim Ueq, Uanis(Na1)
\\sim Ueq, Uanis(Na2) \\sim Ueq: with sigma of 0.005 and sigma for terminal
atoms of 0.01
2. Others
 Fixed Sof: Na1(0.86667) Na2(0.33333) O16(0.8) O16A(0.2) O17(0.65) O17A(0.35)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-x+1/2, y+1, -z+1'
'x+1, -y+1, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1, -x+1, -y+1/2'
'-z+1, -x+1/2, y+1'
'-z+1/2, x+1, -y+1'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1, -x+1'
'y+1, -z+1, -x+1/2'
'-y+1, -z+1/2, x+1'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z'
'-z, -x, -y'
'-z-1/2, x-1/2, y'
'z-1/2, x, -y-1/2'
'z, -x-1/2, y-1/2'
'-y, -z, -x'
'y, -z-1/2, x-1/2'
'-y-1/2, z-1/2, x'
'y-1/2, z, -x-1/2'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'x+1/2, -y, z'
'-x, y, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z, x, y+1/2'
'z, x+1/2, -y'
'z+1/2, -x, y'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z, x'
'-y, z, x+1/2'
'y, z+1/2, -x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.500000 0.500000 0.500000 0.00633(12) Uani 1 6 d S T P . .
U2 U 0.750000 0.750000 0.750000 0.00940(13) Uani 1 6 d S T P . .
Mo1 Mo 0.62817(2) 0.54210(2) 0.51101(2) 0.00922(12) Uani 1 1 d . . . . .
Mo2 Mo 0.56737(2) 0.57946(2) 0.41430(2) 0.00964(12) Uani 1 1 d . . . . .
Mo3 Mo 0.62073(2) 0.71433(2) 0.73462(2) 0.01195(12) Uani 1 1 d . . . . .
Mo4 Mo 0.67404(2) 0.67928(2) 0.83692(2) 0.01296(12) Uani 1 1 d . . . . .
Co1 Co 0.62546(3) 0.62546(3) 0.62546(3) 0.0158(3) Uani 1 3 d S T P . .
Na1 Na 0.58278(9) 0.50336(9) 0.30127(9) 0.0106(5) Uani 0.8667 1 d . U P . .
Na2 Na 0.6621(3) 0.7556(3) 0.9451(3) 0.0152(15) Uani 0.3333 1 d . U P . .
O1 O 0.64642(14) 0.58516(15) 0.55898(15) 0.0135(8) Uani 1 1 d . . . . .
O2 O 0.68084(15) 0.50347(16) 0.50352(16) 0.0175(9) Uani 1 1 d . . . . .
O3 O 0.63304(14) 0.58407(15) 0.45004(15) 0.0126(8) Uani 1 1 d . . . . .
O4 O 0.55022(14) 0.58178(14) 0.49974(14) 0.0093(8) Uani 1 1 d . . . . .
O5 O 0.49862(14) 0.54982(14) 0.41809(14) 0.0102(8) Uani 1 1 d . . . . .
O6 O 0.55187(15) 0.64288(15) 0.40623(15) 0.0154(9) Uani 1 1 d . . . . .
O7 O 0.58671(15) 0.55920(15) 0.35478(15) 0.0140(8) Uani 1 1 d . . . . .
O8 O 0.60357(15) 0.66777(15) 0.68972(15) 0.0167(9) Uani 1 1 d . . . . .
O9 O 0.56912(16) 0.75427(16) 0.73607(17) 0.0197(9) Uani 1 1 d . . . . .
O10 O 0.60944(15) 0.67644(15) 0.79774(15) 0.0168(9) Uani 1 1 d . . . . .
O11 O 0.69582(15) 0.67094(15) 0.75226(15) 0.0130(8) Uani 1 1 d . . . . .
O12 O 0.74470(15) 0.70480(14) 0.83456(14) 0.0130(9) Uani 1 1 d . . . . .
O13 O 0.68449(17) 0.61561(16) 0.84893(16) 0.0218(10) Uani 1 1 d . . . . .
O14 O 0.65372(16) 0.70397(16) 0.89442(15) 0.0188(9) Uani 1 1 d . . . . .
O15 O 0.6607(2) 0.8054(3) 0.9916(2) 0.0561(17) Uani 1 1 d . . . . .
O16 O 0.5704(3) 0.5587(3) 0.2492(3) 0.0398(18) Uani 0.8 1 d . U P . 1
O16A O 0.5474(11) 0.5758(11) 0.2514(10) 0.031(7) Uani 0.2 1 d . U P . 2
O17 O 0.6887(4) 0.6866(4) 1.0014(3) 0.046(2) Uani 0.65 1 d . . P . 1
O17A O 0.7121(6) 0.6619(6) 1.0130(6) 0.035(4) Uani 0.35 1 d . U P . 2
O18 O 0.5572(3) 0.5839(2) 0.7594(2) 0.0565(17) Uani 1 1 d . . . . .
O19 O 0.6288(3) 0.500000 0.750000 0.054(2) Uani 1 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 U1 O4 180.0 33_666 9 ?
O4 U1 O4 63.76(13) 9 5 ?
O4 U1 O4 63.76(13) 9 . ?
O4 U1 O4 63.76(13) 33_666 25_666 ?
O4 U1 O4 180.00(9) 29_666 5 ?
O4 U1 O4 116.24(13) 9 25_666 ?
O4 U1 O4 116.24(13) 33_666 5 ?
O4 U1 O4 116.24(13) 29_666 . ?
O4 U1 O4 116.24(13) 25_666 5 ?
O4 U1 O4 63.76(13) 33_666 29_666 ?
O4 U1 O4 116.24(13) 33_666 . ?
O4 U1 O4 116.24(13) 9 29_666 ?
O4 U1 O4 180.0 25_666 . ?
O4 U1 O4 63.76(13) 25_666 29_666 ?
O4 U1 O4 63.76(13) 5 . ?
O5 U1 O4 117.43(12) 29_666 25_666 ?
O5 U1 O4 117.14(12) 33_666 25_666 ?
O5 U1 O4 62.57(12) 25_666 9 ?
O5 U1 O4 62.57(12) 5 25_666 ?
O5 U1 O4 117.14(12) . 5 ?
O5 U1 O4 64.05(12) 25_666 25_666 ?
O5 U1 O4 115.95(12) 25_666 . ?
O5 U1 O4 115.95(12) . 25_666 ?
O5 U1 O4 64.05(12) 5 5 ?
O5 U1 O4 115.95(12) 9 33_666 ?
O5 U1 O4 62.86(12) 29_666 9 ?
O5 U1 O4 117.14(12) 29_666 33_666 ?
O5 U1 O4 117.13(12) 9 . ?
O5 U1 O4 117.43(12) 33_666 29_666 ?
O5 U1 O4 117.43(12) . 9 ?
O5 U1 O4 62.57(12) 9 29_666 ?
O5 U1 O4 115.95(12) 29_666 5 ?
O5 U1 O4 64.05(12) 29_666 29_666 ?
O5 U1 O4 62.86(12) 25_666 5 ?
O5 U1 O4 62.86(12) 5 33_666 ?
O5 U1 O4 64.05(12) 9 9 ?
O5 U1 O4 117.14(12) 25_666 29_666 ?
O5 U1 O4 117.14(12) 5 9 ?
O5 U1 O4 62.86(12) . 29_666 ?
O5 U1 O4 62.87(12) 33_666 . ?
O5 U1 O4 117.43(12) 25_666 33_666 ?
O5 U1 O4 117.43(12) 5 . ?
O5 U1 O4 62.57(12) . 33_666 ?
O5 U1 O4 64.05(12) . . ?
O5 U1 O4 115.95(12) 33_666 9 ?
O5 U1 O4 64.05(12) 33_666 33_666 ?
O5 U1 O4 62.57(12) 33_666 5 ?
O5 U1 O4 62.86(12) 9 25_666 ?
O5 U1 O4 117.43(12) 9 5 ?
O5 U1 O4 115.95(12) 5 29_666 ?
O5 U1 O4 62.57(12) 29_666 . ?
O5 U1 O5 116.05(6) 33_666 25_666 ?
O5 U1 O5 180.00(9) 25_666 . ?
O5 U1 O5 63.96(6) 33_666 5 ?
O5 U1 O5 63.95(6) 9 25_666 ?
O5 U1 O5 116.05(6) 33_666 29_666 ?
O5 U1 O5 116.05(6) 29_666 25_666 ?
O5 U1 O5 116.05(6) 5 . ?
O5 U1 O5 63.95(6) 5 25_666 ?
O5 U1 O5 180.0 33_666 9 ?
O5 U1 O5 63.96(6) 33_666 . ?
O5 U1 O5 63.95(6) 9 29_666 ?
O5 U1 O5 116.04(6) 9 . ?
O5 U1 O5 180.0 29_666 5 ?
O5 U1 O5 63.95(6) 29_666 . ?
O5 U1 O5 116.05(6) 9 5 ?
O11 U2 O11 115.68(14) . 45_666 ?
O11 U2 O11 115.68(14) 9 41_666 ?
O11 U2 O11 64.32(14) 9 5 ?
O11 U2 O11 64.32(14) 37_666 45_666 ?
O11 U2 O11 115.68(14) 37_666 5 ?
O11 U2 O11 64.32(14) . 9 ?
O11 U2 O11 64.32(14) 45_666 41_666 ?
O11 U2 O11 115.68(14) 37_666 9 ?
O11 U2 O11 64.32(14) . 5 ?
O11 U2 O11 180.0 45_666 9 ?
O11 U2 O11 115.68(14) 45_666 5 ?
O11 U2 O11 115.68(14) . 41_666 ?
O11 U2 O11 64.32(14) 37_666 41_666 ?
O11 U2 O11 180.0 . 37_666 ?
O11 U2 O11 180.0 41_666 5 ?
O11 U2 O12 116.11(12) 37_666 . ?
O11 U2 O12 62.41(12) 41_666 9 ?
O11 U2 O12 62.41(12) 37_666 5 ?
O11 U2 O12 117.60(13) 9 . ?
O11 U2 O12 117.48(12) 45_666 41_666 ?
O11 U2 O12 117.48(12) 5 . ?
O11 U2 O12 63.89(12) 5 5 ?
O11 U2 O12 62.41(12) 9 37_666 ?
O11 U2 O12 62.41(12) . 41_666 ?
O11 U2 O12 117.48(12) 41_666 37_666 ?
O11 U2 O12 63.89(12) 41_666 41_666 ?
O11 U2 O12 62.52(12) 5 37_666 ?
O11 U2 O12 117.48(12) 9 5 ?
O11 U2 O12 62.52(12) . 45_666 ?
O11 U2 O12 63.89(12) 9 9 ?
O11 U2 O12 117.48(12) 37_666 45_666 ?
O11 U2 O12 117.59(12) 5 9 ?
O11 U2 O12 63.89(12) 45_666 45_666 ?
O11 U2 O12 117.59(12) 37_666 41_666 ?
O11 U2 O12 116.11(12) 9 45_666 ?
O11 U2 O12 62.52(12) 9 41_666 ?
O11 U2 O12 117.59(12) 41_666 45_666 ?
O11 U2 O12 116.11(12) 5 41_666 ?
O11 U2 O12 62.41(12) 5 45_666 ?
O11 U2 O12 62.52(12) 45_666 5 ?
O11 U2 O12 117.48(12) . 9 ?
O11 U2 O12 116.11(12) 41_666 5 ?
O11 U2 O12 62.52(12) 37_666 9 ?
O11 U2 O12 63.89(12) . . ?
O11 U2 O12 116.11(12) 45_666 9 ?
O11 U2 O12 62.40(12) 45_666 . ?
O11 U2 O12 116.11(12) . 37_666 ?
O11 U2 O12 62.52(12) 41_666 . ?
O11 U2 O12 63.89(12) 37_666 37_666 ?
O11 U2 O12 117.59(13) 45_666 37_666 ?
O11 U2 O12 117.59(12) . 5 ?
O12 U2 O12 64.08(6) 37_666 5 ?
O12 U2 O12 115.92(6) 37_666 41_666 ?
O12 U2 O12 64.08(6) 41_666 . ?
O12 U2 O12 64.08(6) 45_666 5 ?
O12 U2 O12 115.92(6) 45_666 41_666 ?
O12 U2 O12 115.92(6) 9 5 ?
O12 U2 O12 180.00(18) 45_666 9 ?
O12 U2 O12 180.0 41_666 5 ?
O12 U2 O12 180.00(8) 37_666 . ?
O12 U2 O12 64.08(6) 9 41_666 ?
O12 U2 O12 115.92(6) 9 . ?
O12 U2 O12 115.92(6) 37_666 45_666 ?
O12 U2 O12 115.92(6) 5 . ?
O12 U2 O12 64.08(6) 37_666 9 ?
O12 U2 O12 64.08(6) 45_666 . ?
Mo2 Mo1 U1 63.399(12) . . ?
O1 Mo1 U1 121.08(13) . . ?
O1 Mo1 Mo2 120.94(13) . . ?
O1 Mo1 O3 101.94(17) . . ?
O1 Mo1 O4 92.48(16) . . ?
O1 Mo1 O4 99.17(17) . 9 ?
O1 Mo1 O5 161.95(16) . 29_666 ?
O2 Mo1 U1 124.51(14) . . ?
O2 Mo1 Mo2 119.76(14) . . ?
O2 Mo1 O1 103.94(19) . . ?
O2 Mo1 O3 100.73(18) . . ?
O2 Mo1 O4 163.32(17) . . ?
O2 Mo1 O4 103.07(18) . 9 ?
O2 Mo1 O5 94.11(17) . 29_666 ?
O3 Mo1 U1 99.86(11) . . ?
O3 Mo1 Mo2 36.48(11) . . ?
O3 Mo1 O4 72.45(14) . . ?
O3 Mo1 O5 73.97(15) . 29_666 ?
O4 Mo1 U1 44.97(9) . . ?
O4 Mo1 U1 43.27(11) 9 . ?
O4 Mo1 Mo2 46.38(9) . . ?
O4 Mo1 Mo2 106.67(11) 9 . ?
O4 Mo1 O3 143.12(16) 9 . ?
O4 Mo1 O4 76.78(19) 9 . ?
O4 Mo1 O5 76.60(15) 9 29_666 ?
O5 Mo1 U1 44.83(9) 29_666 . ?
O5 Mo1 Mo2 46.43(9) 29_666 . ?
O5 Mo1 O4 69.49(13) 29_666 . ?
U1 Mo2 Na1 103.80(4) . 33_666 ?
U1 Mo2 Na1 104.65(4) . . ?
Mo1 Mo2 U1 63.790(12) . . ?
Mo1 Mo2 Na1 115.71(4) . . ?
Mo1 Mo2 Na1 120.56(4) . 33_666 ?
Na1 Mo2 Na1 123.50(4) . 33_666 ?
O3 Mo2 U1 99.85(11) . . ?
O3 Mo2 Mo1 36.08(11) . . ?
O3 Mo2 Na1 109.20(12) . . ?
O3 Mo2 Na1 112.59(12) . 33_666 ?
O3 Mo2 O4 72.74(14) . . ?
O3 Mo2 O5 73.29(15) . 29_666 ?
O3 Mo2 O5 143.54(15) . . ?
O4 Mo2 U1 45.15(9) . . ?
O4 Mo2 Mo1 47.09(9) . . ?
O4 Mo2 Na1 81.73(10) . 33_666 ?
O4 Mo2 Na1 147.64(10) . . ?
O5 Mo2 U1 45.09(9) 29_666 . ?
O5 Mo2 U1 43.69(11) . . ?
O5 Mo2 Mo1 107.48(11) . . ?
O5 Mo2 Mo1 46.04(10) 29_666 . ?
O5 Mo2 Na1 79.83(10) 29_666 . ?
O5 Mo2 Na1 85.71(12) . . ?
O5 Mo2 Na1 82.61(12) . 33_666 ?
O5 Mo2 Na1 147.88(10) 29_666 33_666 ?
O5 Mo2 O4 69.71(13) 29_666 . ?
O5 Mo2 O4 77.32(14) . . ?
O5 Mo2 O5 77.17(17) . 29_666 ?
O6 Mo2 U1 121.89(13) . . ?
O6 Mo2 Mo1 121.18(14) . . ?
O6 Mo2 Na1 117.41(14) . . ?
O6 Mo2 Na1 18.81(14) . 33_666 ?
O6 Mo2 O3 101.87(18) . . ?
O6 Mo2 O4 92.77(16) . . ?
O6 Mo2 O5 99.87(17) . . ?
O6 Mo2 O5 162.48(16) . 29_666 ?
O7 Mo2 U1 122.70(13) . . ?
O7 Mo2 Mo1 118.92(13) . . ?
O7 Mo2 Na1 115.71(14) . 33_666 ?
O7 Mo2 Na1 18.23(13) . . ?
O7 Mo2 O3 101.12(17) . . ?
O7 Mo2 O4 162.33(16) . . ?
O7 Mo2 O5 92.72(16) . 29_666 ?
O7 Mo2 O5 101.16(17) . . ?
O7 Mo2 O6 104.78(18) . . ?
U2 Mo3 Na2 102.05(11) . 41_666 ?
Mo4 Mo3 U2 63.685(13) . . ?
Mo4 Mo3 Na2 113.86(10) . 41_666 ?
O8 Mo3 U2 120.39(13) . . ?
O8 Mo3 Mo4 118.71(14) . . ?
O8 Mo3 Na2 122.60(17) . 41_666 ?
O8 Mo3 O10 100.13(18) . . ?
O8 Mo3 O11 100.31(18) . 9 ?
O8 Mo3 O11 90.58(17) . . ?
O8 Mo3 O12 160.13(17) . 41_666 ?
O9 Mo3 U2 126.37(15) . . ?
O9 Mo3 Mo4 120.58(15) . . ?
O9 Mo3 Na2 24.33(18) . 41_666 ?
O9 Mo3 O8 103.8(2) . . ?
O9 Mo3 O10 99.94(19) . . ?
O9 Mo3 O11 103.57(19) . 9 ?
O9 Mo3 O11 165.11(18) . . ?
O9 Mo3 O12 95.98(18) . 41_666 ?
O10 Mo3 U2 100.55(12) . . ?
O10 Mo3 Mo4 36.87(12) . . ?
O10 Mo3 Na2 108.53(16) . 41_666 ?
O10 Mo3 O11 73.16(15) . . ?
O10 Mo3 O12 73.94(15) . 41_666 ?
O11 Mo3 U2 43.43(12) 9 . ?
O11 Mo3 U2 45.11(10) . . ?
O11 Mo3 Mo4 46.62(10) . . ?
O11 Mo3 Mo4 107.11(12) 9 . ?
O11 Mo3 Na2 144.67(15) . 41_666 ?
O11 Mo3 Na2 84.46(16) 9 41_666 ?
O11 Mo3 O10 143.98(17) 9 . ?
O11 Mo3 O11 77.3(2) 9 . ?
O11 Mo3 O12 76.79(15) 9 41_666 ?
O12 Mo3 U2 45.06(10) 41_666 . ?
O12 Mo3 Mo4 46.27(10) 41_666 . ?
O12 Mo3 Na2 76.99(14) 41_666 41_666 ?
O12 Mo3 O11 69.57(14) 41_666 . ?
U2 Mo4 Na2 100.55(11) . 45_666 ?
Mo3 Mo4 U2 63.348(13) . . ?
Mo3 Mo4 Na2 118.46(10) . 45_666 ?
Mo3 Mo4 Na2 118.94(11) . . ?
Na2 Mo4 U2 105.84(11) . . ?
Na2 Mo4 Na2 122.57(11) . 45_666 ?
O10 Mo4 U2 99.57(11) . . ?
O10 Mo4 Mo3 36.24(11) . . ?
O10 Mo4 Na2 111.50(16) . . ?
O10 Mo4 Na2 113.04(16) . 45_666 ?
O10 Mo4 O11 73.07(15) . . ?
O10 Mo4 O12 72.56(15) . 41_666 ?
O11 Mo4 U2 44.88(10) . . ?
O11 Mo4 Mo3 47.10(10) . . ?
O11 Mo4 Na2 78.58(14) . 45_666 ?
O11 Mo4 Na2 149.47(15) . . ?
O12 Mo4 U2 43.53(11) . . ?
O12 Mo4 U2 44.95(10) 41_666 . ?
O12 Mo4 Mo3 45.29(10) 41_666 . ?
O12 Mo4 Mo3 106.88(11) . . ?
O12 Mo4 Na2 144.22(14) 41_666 45_666 ?
O12 Mo4 Na2 83.10(15) 41_666 . ?
O12 Mo4 Na2 85.12(16) . . ?
O12 Mo4 Na2 80.40(15) . 45_666 ?
O12 Mo4 O10 143.10(16) . . ?
O12 Mo4 O11 76.64(15) . . ?
O12 Mo4 O11 69.25(14) 41_666 . ?
O12 Mo4 O12 77.38(18) . 41_666 ?
O13 Mo4 U2 122.34(15) . . ?
O13 Mo4 Mo3 120.51(15) . . ?
O13 Mo4 Na2 114.99(18) . . ?
O13 Mo4 Na2 22.46(18) . 45_666 ?
O13 Mo4 O10 101.21(19) . . ?
O13 Mo4 O11 92.57(17) . . ?
O13 Mo4 O12 161.74(17) . 41_666 ?
O13 Mo4 O12 100.69(19) . . ?
O13 Mo4 O14 104.7(2) . . ?
O14 Mo4 U2 122.57(14) . . ?
O14 Mo4 Mo3 119.72(14) . . ?
O14 Mo4 Na2 17.36(18) . . ?
O14 Mo4 Na2 118.21(17) . 45_666 ?
O14 Mo4 O10 101.71(18) . . ?
O14 Mo4 O11 162.70(17) . . ?
O14 Mo4 O12 93.47(17) . 41_666 ?
O14 Mo4 O12 100.97(18) . . ?
O1 Co1 O1 86.11(15) 9 . ?
O1 Co1 O1 86.10(15) 5 . ?
O1 Co1 O1 86.11(16) 9 5 ?
O8 Co1 O1 92.20(15) 5 9 ?
O8 Co1 O1 177.80(16) 5 5 ?
O8 Co1 O1 95.20(15) 5 . ?
O8 Co1 O1 92.20(15) . 5 ?
O8 Co1 O1 92.20(15) 9 . ?
O8 Co1 O1 177.80(16) 9 9 ?
O8 Co1 O1 177.80(16) . . ?
O8 Co1 O1 95.19(15) . 9 ?
O8 Co1 O1 95.19(15) 9 5 ?
O8 Co1 O8 86.54(17) . 9 ?
O8 Co1 O8 86.54(16) . 5 ?
O8 Co1 O8 86.54(16) 9 5 ?
Mo2 Na1 Mo2 64.95(4) . 29_666 ?
Na1 Na1 Mo2 149.18(13) 16_455 . ?
Na1 Na1 Mo2 145.57(14) 16_455 29_666 ?
Na1 Na1 O17 95.4(2) 16_455 48_546 ?
O2 Na1 Mo2 76.50(12) 33_666 . ?
O2 Na1 Mo2 78.85(12) 33_666 29_666 ?
O2 Na1 Na1 101.36(12) 33_666 16_455 ?
O2 Na1 O16A 78.6(7) 33_666 . ?
O2 Na1 O16A 72.8(6) 33_666 16_455 ?
O2 Na1 O17 161.9(3) 33_666 48_546 ?
O6 Na1 Mo2 15.52(11) 29_666 29_666 ?
O6 Na1 Mo2 79.73(13) 29_666 . ?
O6 Na1 Na1 131.08(19) 29_666 16_455 ?
O6 Na1 O2 86.47(17) 29_666 33_666 ?
O6 Na1 O16 85.8(2) 29_666 16_455 ?
O6 Na1 O16A 162.6(7) 29_666 . ?
O6 Na1 O16A 82.5(6) 29_666 16_455 ?
O6 Na1 O17 77.4(2) 29_666 48_546 ?
O6 Na1 O17A 93.7(5) 29_666 48_546 ?
O7 Na1 Mo2 15.42(11) . . ?
O7 Na1 Mo2 76.84(13) . 29_666 ?
O7 Na1 Na1 137.45(19) . 16_455 ?
O7 Na1 O2 88.04(17) . 33_666 ?
O7 Na1 O6 90.49(18) . 29_666 ?
O7 Na1 O16 172.5(3) . 16_455 ?
O7 Na1 O16A 159.9(6) . 16_455 ?
O7 Na1 O16A 80.3(7) . . ?
O7 Na1 O17 84.1(2) . 48_546 ?
O7 Na1 O17A 88.8(5) . 48_546 ?
O16 Na1 Mo2 98.5(2) 16_455 29_666 ?
O16 Na1 Mo2 98.1(2) . . ?
O16 Na1 Mo2 162.1(2) . 29_666 ?
O16 Na1 Mo2 157.2(2) 16_455 . ?
O16 Na1 Na1 47.8(2) 16_455 16_455 ?
O16 Na1 Na1 51.1(2) . 16_455 ?
O16 Na1 O2 92.1(3) . 33_666 ?
O16 Na1 O2 85.2(3) 16_455 33_666 ?
O16 Na1 O6 177.6(3) . 29_666 ?
O16 Na1 O7 87.6(2) . . ?
O16 Na1 O16 96.0(3) . 16_455 ?
O16 Na1 O16A 98.8(6) . 16_455 ?
O16 Na1 O16A 12.8(6) 16_455 16_455 ?
O16 Na1 O17 101.4(3) 16_455 48_546 ?
O16 Na1 O17 103.8(3) . 48_546 ?
O16 Na1 O17A 87.7(5) . 48_546 ?
O16A Na1 Mo2 148.2(7) . 29_666 ?
O16A Na1 Mo2 145.2(6) 16_455 . ?
O16A Na1 Mo2 88.2(7) . . ?
O16A Na1 Mo2 93.2(6) 16_455 29_666 ?
O16A Na1 Na1 61.6(7) . 16_455 ?
O16A Na1 Na1 55.3(6) 16_455 16_455 ?
O16A Na1 O16A 101.1(9) . 16_455 ?
O16A Na1 O17 112.5(6) 16_455 48_546 ?
O16A Na1 O17 115.9(7) . 48_546 ?
O17 Na1 Mo2 92.5(2) 48_546 . ?
O17 Na1 Mo2 83.5(2) 48_546 29_666 ?
O17A Na1 Mo2 100.4(5) 48_546 . ?
O17A Na1 Mo2 100.5(5) 48_546 29_666 ?
O17A Na1 Na1 80.9(5) 48_546 16_455 ?
O17A Na1 O16 97.9(5) 48_546 16_455 ?
O17A Na1 O16A 100.8(8) 48_546 . ?
O17A Na1 O16A 110.4(7) 48_546 16_455 ?
O17A Na1 O17 17.0(5) 48_546 48_546 ?
Mo3 Na2 Mo4 63.34(11) 45_666 41_666 ?
Mo4 Na2 Mo3 65.10(12) . 45_666 ?
Mo4 Na2 Mo4 64.75(12) . 41_666 ?
O9 Na2 Mo3 18.39(14) 45_666 45_666 ?
O9 Na2 Mo4 78.4(2) 45_666 41_666 ?
O9 Na2 Mo4 80.3(2) 45_666 . ?
O9 Na2 O13 86.5(3) 45_666 41_666 ?
O9 Na2 O16 161.6(4) 45_666 23_456 ?
O9 Na2 O16A 175.2(8) 45_666 23_456 ?
O9 Na2 O17 83.8(3) 45_666 . ?
O13 Na2 Mo3 74.5(2) 41_666 45_666 ?
O13 Na2 Mo4 80.6(2) 41_666 . ?
O13 Na2 Mo4 16.95(13) 41_666 41_666 ?
O13 Na2 O16 78.5(3) 41_666 23_456 ?
O13 Na2 O16A 89.4(8) 41_666 23_456 ?
O13 Na2 O17 168.9(4) 41_666 . ?
O14 Na2 Mo3 79.9(2) . 45_666 ?
O14 Na2 Mo4 75.2(2) . 41_666 ?
O14 Na2 Mo4 15.63(16) . . ?
O14 Na2 O9 93.8(3) . 45_666 ?
O14 Na2 O13 89.3(3) . 41_666 ?
O14 Na2 O16 75.6(3) . 23_456 ?
O14 Na2 O16A 83.6(8) . 23_456 ?
O14 Na2 O17 85.9(3) . . ?
O15 Na2 Mo3 106.7(3) . 45_666 ?
O15 Na2 Mo4 103.6(3) . 41_666 ?
O15 Na2 Mo4 167.6(4) . . ?
O15 Na2 O9 93.6(4) . 45_666 ?
O15 Na2 O13 88.3(4) . 41_666 ?
O15 Na2 O14 172.1(5) . . ?
O15 Na2 O16 96.6(4) . 23_456 ?
O15 Na2 O16A 88.9(8) . 23_456 ?
O15 Na2 O17 97.8(4) . . ?
O16 Na2 Mo3 143.4(3) 23_456 45_666 ?
O16 Na2 Mo4 86.7(2) 23_456 . ?
O16 Na2 Mo4 84.3(2) 23_456 41_666 ?
O16A Na2 Mo4 97.0(8) 23_456 41_666 ?
O16A Na2 Mo4 96.5(7) 23_456 . ?
O17 Na2 Mo3 94.8(3) . 45_666 ?
O17 Na2 Mo4 92.3(3) . . ?
O17 Na2 Mo4 152.9(3) . 41_666 ?
O17 Na2 O16 109.8(4) . 23_456 ?
Mo1 O1 Co1 147.3(2) . . ?
Mo1 O2 Na1 138.1(2) . 29_666 ?
Mo1 O3 Mo2 107.44(17) . . ?
Mo1 O4 U1 94.52(13) . . ?
Mo1 O4 U1 104.79(15) 5 . ?
Mo1 O4 Mo1 132.59(18) 5 . ?
Mo1 O4 Mo2 132.96(18) 5 . ?
Mo2 O4 U1 94.76(13) . . ?
Mo2 O4 Mo1 86.53(13) . . ?
Mo1 O5 U1 95.63(13) 33_666 . ?
Mo1 O5 Mo2 87.53(13) 33_666 33_666 ?
Mo2 O5 U1 103.62(15) . . ?
Mo2 O5 U1 94.83(13) 33_666 . ?
Mo2 O5 Mo1 133.01(18) . 33_666 ?
Mo2 O5 Mo2 131.86(19) . 33_666 ?
Mo2 O6 Na1 145.7(2) . 33_666 ?
Mo2 O7 Na1 146.3(2) . . ?
Mo3 O8 Co1 146.8(2) . . ?
Mo3 O9 Na2 137.3(3) . 41_666 ?
Mo3 O10 Mo4 106.89(18) . . ?
Mo3 O11 U2 94.04(13) . . ?
Mo3 O11 U2 104.56(16) 5 . ?
Mo3 O11 Mo3 132.54(19) 5 . ?
Mo3 O11 Mo4 133.57(19) 5 . ?
Mo4 O11 U2 94.85(14) . . ?
Mo4 O11 Mo3 86.28(13) . . ?
Mo3 O12 U2 95.76(14) 45_666 . ?
Mo3 O12 Mo4 88.45(14) 45_666 45_666 ?
Mo4 O12 U2 95.18(14) 45_666 . ?
Mo4 O12 U2 103.85(16) . . ?
Mo4 O12 Mo3 132.30(19) . 45_666 ?
Mo4 O12 Mo4 131.34(19) . 45_666 ?
Mo4 O13 Na2 140.6(3) . 45_666 ?
Mo4 O14 Na2 147.0(3) . . ?
Na1 O16 Na1 81.2(3) . 16_455 ?
Na1 O16 Na2 138.7(3) 16_455 20_645 ?
Na1 O16 Na2 139.9(4) . 20_645 ?
Na1 O16A Na1 63.0(7) . 16_455 ?
Na2 O16A Na1 140.3(12) 20_645 . ?
Na2 O16A Na1 134.7(12) 20_645 16_455 ?
Na2 O17 Na1 141.0(4) . 42_655 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 O4 2.491(4) 33_666 ?
U1 O4 2.491(4) . ?
U1 O4 2.491(4) 5 ?
U1 O4 2.491(4) 9 ?
U1 O4 2.491(4) 29_666 ?
U1 O4 2.491(4) 25_666 ?
U1 O5 2.489(4) 33_666 ?
U1 O5 2.489(4) . ?
U1 O5 2.489(4) 5 ?
U1 O5 2.489(4) 9 ?
U1 O5 2.489(4) 29_666 ?
U1 O5 2.489(4) 25_666 ?
U2 O11 2.489(4) . ?
U2 O11 2.489(4) 5 ?
U2 O11 2.489(4) 41_666 ?
U2 O11 2.489(4) 37_666 ?
U2 O11 2.489(4) 45_666 ?
U2 O11 2.489(4) 9 ?
U2 O12 2.493(4) 37_666 ?
U2 O12 2.493(4) . ?
U2 O12 2.493(4) 5 ?
U2 O12 2.493(4) 45_666 ?
U2 O12 2.493(4) 9 ?
U2 O12 2.493(4) 41_666 ?
Mo1 Mo2 3.1201(7) . ?
Mo1 O1 1.739(4) . ?
Mo1 O2 1.707(4) . ?
Mo1 O3 1.926(4) . ?
Mo1 O4 1.922(4) 9 ?
Mo1 O4 2.290(4) . ?
Mo1 O5 2.248(4) 29_666 ?
Mo2 Na1 3.560(2) . ?
Mo2 Na1 3.601(2) 33_666 ?
Mo2 O3 1.945(4) . ?
Mo2 O4 2.263(4) . ?
Mo2 O5 2.263(4) 29_666 ?
Mo2 O5 1.946(4) . ?
Mo2 O6 1.708(4) . ?
Mo2 O7 1.708(4) . ?
Mo3 Mo4 3.1299(7) . ?
Mo3 Na2 3.644(7) 41_666 ?
Mo3 O8 1.737(4) . ?
Mo3 O9 1.695(4) . ?
Mo3 O10 1.934(4) . ?
Mo3 O11 1.919(4) 9 ?
Mo3 O11 2.298(4) . ?
Mo3 O12 2.225(4) 41_666 ?
Mo4 Na2 3.710(7) 45_666 ?
Mo4 Na2 3.452(7) . ?
Mo4 O10 1.963(4) . ?
Mo4 O11 2.280(4) . ?
Mo4 O12 1.951(4) . ?
Mo4 O12 2.262(4) 41_666 ?
Mo4 O13 1.704(4) . ?
Mo4 O14 1.708(4) . ?
Co1 O1 2.090(4) . ?
Co1 O1 2.090(4) 9 ?
Co1 O1 2.090(4) 5 ?
Co1 O8 2.077(4) 9 ?
Co1 O8 2.077(4) 5 ?
Co1 O8 2.077(4) . ?
Na1 Na1 2.668(5) 16_455 ?
Na1 O2 2.294(5) 33_666 ?
Na1 O6 2.059(5) 29_666 ?
Na1 O7 2.010(5) . ?
Na1 O16 2.100(8) 16_455 ?
Na1 O16 1.999(8) . ?
Na1 O16A 2.63(3) 16_455 ?
Na1 O16A 2.46(3) . ?
Na1 O17 2.708(10) 48_546 ?
Na1 O17A 2.097(15) 48_546 ?
Na2 O9 2.213(8) 45_666 ?
Na2 O13 2.233(8) 41_666 ?
Na2 O14 1.892(8) . ?
Na2 O15 1.767(9) . ?
Na2 O16 2.718(10) 23_456 ?
Na2 O16A 2.26(3) 23_456 ?
Na2 O17 2.413(12) . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 Mo1 O1 Co1 7.4(5) . . . . ?
U1 Mo1 O2 Na1 -10.9(4) . . . 29_666 ?
U1 Mo2 O6 Na1 -17.2(5) . . . 33_666 ?
U1 Mo2 O7 Na1 8.9(5) . . . . ?
U2 Mo3 O8 Co1 -15.9(5) . . . . ?
U2 Mo3 O9 Na2 2.2(5) . . . 41_666 ?
U2 Mo4 O13 Na2 15.4(5) . . . 45_666 ?
U2 Mo4 O14 Na2 -16.7(7) . . . . ?
Mo1 Mo2 O6 Na1 -93.8(4) . . . 33_666 ?
Mo1 Mo2 O7 Na1 84.7(4) . . . . ?
Mo2 Mo1 O1 Co1 83.1(4) . . . . ?
Mo2 Mo1 O2 Na1 -87.4(3) . . . 29_666 ?
Mo3 Mo4 O13 Na2 91.3(5) . . . 45_666 ?
Mo3 Mo4 O14 Na2 -92.3(6) . . . . ?
Mo3 Na2 O14 Mo4 -18.6(6) 45_666 . . . ?
Mo4 Mo3 O8 Co1 -90.6(4) . . . . ?
Mo4 Mo3 O9 Na2 80.4(4) . . . 41_666 ?
Mo4 Na2 O14 Mo4 46.3(6) 41_666 . . . ?
Na1 Mo2 O6 Na1 113.9(4) . . . 33_666 ?
Na1 Mo2 O7 Na1 -119.7(4) 33_666 . . . ?
Na2 Mo3 O8 Co1 115.5(4) 41_666 . . . ?
Na2 Mo4 O13 Na2 -115.3(4) . . . 45_666 ?
Na2 Mo4 O14 Na2 109.4(6) 45_666 . . . ?
O1 Mo1 O2 Na1 133.8(3) . . . 29_666 ?
O2 Mo1 O1 Co1 -138.8(4) . . . . ?
O3 Mo1 O1 Co1 116.8(4) . . . . ?
O3 Mo1 O2 Na1 -120.9(3) . . . 29_666 ?
O3 Mo2 O6 Na1 -126.9(4) . . . 33_666 ?
O3 Mo2 O7 Na1 118.3(4) . . . . ?
O4 Mo1 O1 Co1 -32.7(4) 9 . . . ?
O4 Mo1 O1 Co1 44.3(4) . . . . ?
O4 Mo1 O2 Na1 -56.7(8) . . . 29_666 ?
O4 Mo1 O2 Na1 30.8(4) 9 . . 29_666 ?
O4 Mo2 O6 Na1 -53.9(4) . . . 33_666 ?
O4 Mo2 O7 Na1 50.6(8) . . . . ?
O5 Mo1 O1 Co1 42.0(8) 29_666 . . . ?
O5 Mo1 O2 Na1 -46.4(3) 29_666 . . 29_666 ?
O5 Mo2 O6 Na1 23.7(5) . . . 33_666 ?
O5 Mo2 O6 Na1 -54.9(8) 29_666 . . 33_666 ?
O5 Mo2 O7 Na1 44.8(4) 29_666 . . . ?
O5 Mo2 O7 Na1 -32.6(5) . . . . ?
O6 Mo2 O7 Na1 -136.1(4) . . . . ?
O7 Mo2 O6 Na1 128.1(4) . . . 33_666 ?
O8 Mo3 O9 Na2 -143.6(4) . . . 41_666 ?
O9 Mo3 O8 Co1 132.4(4) . . . . ?
O9 Na2 O14 Mo4 -30.6(7) 45_666 . . . ?
O10 Mo3 O8 Co1 -124.6(4) . . . . ?
O10 Mo3 O9 Na2 113.3(4) . . . 41_666 ?
O10 Mo4 O13 Na2 124.4(4) . . . 45_666 ?
O10 Mo4 O14 Na2 -126.2(6) . . . . ?
O11 Mo3 O8 Co1 -51.6(4) . . . . ?
O11 Mo3 O8 Co1 25.6(5) 9 . . . ?
O11 Mo3 O9 Na2 52.3(9) . . . 41_666 ?
O11 Mo3 O9 Na2 -39.2(5) 9 . . 41_666 ?
O11 Mo4 O13 Na2 51.2(5) . . . 45_666 ?
O11 Mo4 O14 Na2 -55.8(9) . . . . ?
O12 Mo3 O8 Co1 -54.1(8) 41_666 . . . ?
O12 Mo3 O9 Na2 38.6(4) 41_666 . . 41_666 ?
O12 Mo4 O13 Na2 -25.7(5) . . . 45_666 ?
O12 Mo4 O13 Na2 56.4(8) 41_666 . . 45_666 ?
O12 Mo4 O14 Na2 24.5(6) . . . . ?
O12 Mo4 O14 Na2 -53.3(6) 41_666 . . . ?
O13 Mo4 O14 Na2 128.7(6) . . . . ?
O13 Na2 O14 Mo4 55.8(6) 41_666 . . . ?
O14 Mo4 O13 Na2 -130.2(5) . . . 45_666 ?
O16 Na2 O14 Mo4 134.2(6) 23_456 . . . ?
O16A Na2 O14 Mo4 145.3(9) 23_456 . . . ?
O17 Na2 O14 Mo4 -114.2(6) . . . . ?
